# SUMMARY OF HOT AND COLD PROCESSING

## Presentation on theme: "SUMMARY OF HOT AND COLD PROCESSING"— Presentation transcript:

SUMMARY OF HOT AND COLD PROCESSING
In hot working, significant shape change can be accomplished In cold working, strength can be increased during shape change In cold working, little or no waste-some operations are near net shape or net shape process By cold working the parts require little or no subsequent machining

ROLLING Deformation process in which work thickness is reduced by compressive forces exerted by two opposing rolls. The rotating rolls perform two main functions: Pull the work into the gap between them by friction between workpart and rolls Simultaneously squeeze the work to reduce cross section

TYPES OF ROLLING By geometry of work:
-Flat rolling-used to reduce thickness of a rectangular cross section -Shape rolling-a square cross-section is formed into a shape such as an I-beam By temperature of work: -Hot rolling-most common due to the large amount of deformation required -Cold rolling-produces finished sheet and plate stock

Some of the steel products made in a Rolling Mill

ROLLING GEOMETRY Draft=amount of thickness reduction
Where d=draft; to = starting thickness; and tf = final thickness Reduction=draft expressed as a fraction of starting short thickness Side view of flat rolling, indicating before and after thicknesses, work velocities, angle of contact with rolls, and other features Where r=reduction

SHAPE ROLLING Work is deformed into a contoured cross-section rather than flat (rectangular) Accomplished by passing work through rolls that have the reverse of desired shape Products include: -Construction shapes such as I-beams, L-beams, and U-channels -Rails for railroad tracks -Round and square bars and rods

ROLLING MILLS Equipment is massive and expensive.
Two High Rolling Mill ThreeHigh Rolling Mill Cluster Rolling Mill: Multiple Rolling Mills allow even smaller rolling mills Four High Rolling Mill Tandem Rolling Mill

THREAD ROLLING Bulk deformation process used to form threads on cylindirical parts by rolling them between two dies. Most important commercial process fr mass producing bolts and screws Performed by cold working in thread rolling machines Advantages over thread cutting (machining): -Higher production rates -Better material utilization -Stronger threads due to work hardening -Better fatigue resistance due to compressive stresses introduced by rolling

RING ROLLING Deformation process in which a thick-walled ring of smaller diameter is rolled into a thin-walled ring of larger diameter As thick-walled ring is compressed, deformed metal elongates, causing diameter of ring to be enlarged Hot working process for large rings and cold working process for smaller rings Applications: ball and roller bearing races, steel tires for railroads wheels, and rings for pipes, pressure vessels, and rotating machiners Advantages: material savings, ideal grain orientation, strengthening through cold working

RING ROLLING

FORGING Deformation process in which work is compressed between two dies Oldest of the metal forming operations, dating from about 5000 B C Components: engine crankshafts, connecting rods, gears, aircraft structural components, jet engine, turbine parts In addition, basic metals industries use forging to establish basic form of large components that are subsequently machined to final shape and size. Classification of Forging Operations •Cold vs. hot forging: Hot or warm forging –most common, due to the significant deformation and the need to reduce strength and increase ductility of work metal Cold forging - advantage is increased strength that results from strain hardening. • Impact vs. press forging: Forge hammer - applies an impact load Forge press - applies gradual pressure

TYPES OF FORGING DIES OPEN DIE FORGING Compression of workpart with cylindrical cross-section between two flat dies. •Similar to compression test •Deformation operation reduces height and increases diameter of work •Common names include upsetting or upset forging If no friction occurs between work and die surfaces, then homogeneous deformation occurs, so that radial flow is uniform throughout workpart height and true strain is given by: where ho= starting height; and h = height at some point during compression. At h = final value hf, true strain is maximum value

TYPES OF FORGING DIES Actual Deformation of a cylindiricak workpart in open-die forging, show,no pronounced barreling:

TYPES OF FORGING DIES Friction between work and die surfaces constrains lateral flow of work, resulting in barreling effect. In hot open-die forging, effect is even more pronounced due to heat transfer at and near die surfaces, which cools the metal and increases its resistance to deformation Actual deformation of a cylindrical workpart in open-die forging, showing pronounced barreling: (1) start of process, (2) partial deformation, and (3) final shape

TYPES OF FORGING DIES Sequence in impression-die forging:
(1) just prior to initial contact with raw workpiece, (2) partial compression, and (3) final die closure, causing flash to form in gap between die plates IMPRESSION DIE FORGING Compression of workpart by dies with inverse of desired part shape •Flash is formed by metal that flows beyond die cavity into small gap between die plates •Flash must be later trimmed from part, but it serves an important function during compression: As flash forms, friction resists continued metal flow into gap, constraining material to fill die cavity. In hot forging, metal flow is further restricted by cooling against die plates

Impression-Die Forging Practice
Several forming steps often required, with separate die cavities for each step Beginning steps redistribute metal for more uniform deformation and desired metallurgical structure in subsequent steps Final steps bring the part to its final geometry Impression-die forging is often performed manually by skilled operator under adverse conditions

Advantages compared to machining from solid stock: Higher production rates Conservation of metal (less waste) Greater strength Favorable grain orientation in the metal Limitations: Not capable of close tolerances Machining often required to achieve accuracies and features needed, such as holes, threads, and mating surfaces that fit with other components

TYPES OF FORGING DIES Flashless forging:
(1) just before initial contact with workpiece, (2) partial compression, and (3) final punch and die closure Compression of work in punch and die tooling whose cavity does allow for flash Starting workpart volume must equal die cavity volume within very close tolerance. Process control more demanding than impression-die forging Best suited to part geometries that are simple and symmetrical Often classified as a precision forging process

Forging Hammers (Drop Hammers)
Apply an impact load against workpart - two types: Gravity drop hammers - impact energy from falling weight of a heavy ram Power drop hammers - accelerate the ram by pressurized air or steam Disadvantage: impact energy transmitted through anvil into floor of building Most commonly used for impression-die forging

(photo courtesy of Chambersburg Engineering Company)
Drop forging hammer, fed by conveyor and heating units at the right of the scene (photo courtesy of Chambersburg Engineering Company) Diagram showing details of a drop hammer for impression-die forging

FORGING PRESSES Apply gradual pressure to accomplish compression operation - types: Mechanical presses - converts rotation of drive motor into linear motion of ram Hydraulic presses - hydraulic piston actuates ram Screw presses - screw mechanism drives ram

Upsetting and Heading Forging process used to form heads on nails, bolts, and similar hardware products More parts produced by upsetting than any other forging operation Performed cold, warm, or hot on machines called headers or formers Wire or bar stock is fed into machine, end is headed, then piece is cut to length For bolts and screws, thread rolling is then used to form threads

Upsetting and Heading An upset forging operation to form a head on a bolt or similar hardware item The cycle consists of: (1) wire stock is fed to the stop (2) gripping dies close on the stock and the stop is retracted (3) punch moves forward (4) bottoms to form the head Examples of heading (upset forging) operations: (a) heading a nail using open dies (b) round head formed by punch (c) and (d) two common head styles for screws formed by die (e) carriage bolt head formed by punch and die

EXTRUSION Compression forming process in which the work metal is forced to flow through a die opening to produce a desired cross-sectional shape Process is similar to squeezing toothpaste out of a toothpaste tube In general, extrusion is used to produce long parts of uniform cross-sections Two basic types of extrusion: Direct extrusion Indirect extrusion

DIRECT EXTRUSION Also called forward extrusion
•As ram approaches die opening, a small portion of billet remains that cannot be forced through die opening •This extra portion, called the butt, must be separated from extruded product by cutting it just beyond the die exit •Starting billet cross section usually round, but final shape is determined by die opening

DIRECT EXTRUSION (a) Direct extrusion to produce a hollow or semi-hollow cross-section; (b) hollow and (c) semi-hollow cross- sections

INDIRECT EXTRUSION Also called backward extrusion and reverse extrusion Limitations of indirect extrusion are imposed by the lower rigidity of hollow ram and difficulty in supporting extruded product as it exits die Indirect extrusion to produce (a) a solid cross-section and (b) a hollow cross-section

Variety of shapes possible, especially in hot extrusion Limitation: part cross-section must be uniform throughout length Grain structure and strength enhanced in cold and warm extrusion Close tolerances possible, especially in cold extrusion In some operations, little or no waste of material Hot vs. Cold Extrusion •Hot extrusion - prior heating of billet to above its recrystallization temperature This reduces strength and increases ductility of the metal, permitting more size reductions and more complex shapes •Cold extrusion - generally used to produce discrete parts The term impact extrusion is used to indicate high speed cold extrusion

EXTRUSION RATIO Also called the reduction ratio, it is defined as
where rx = extrusion ratio; Ao = cross-sectional area of the starting billet; and Af = final cross-sectional area of the extruded section Applies to both direct and indirect extrusion

(a) Definition of die angle in direct extrusion;
(b) effect of die angle on ram force